TOOL STEEL are high quality steels made to controlledchemical composition and processed to develop propertiesuseful for working and shaping of other materials.The Carbon content in them is between 0.1 -1.6% . Toolsteel also contain alloying elementslike, Chromium, Molybdenum and Vanadium.Tool steel offers better durability, strength, corrosionresistance and temperature stability, as compared to theConstruction & Engg. Steel.These are used in applications such as Blanking, dieforging, forming, extrusion and plastic molding etc..
SHOCK-RESISTING TOOL STEELSCarbon content = 0.5-0.6%. Alloying elements – Cr, W , Mo.These are characterized by good toughness, hardness andimproved hardenability. These steels are generally, water or oil-hardened.“Low temperature Tempering” is carried out where, toughnessand hardness of the tool steel are of primeimportance, otherwise “High temperature Tempering” ispreferred.Silicon-manganese steels (0.55% C, 2.0% Si, 1.0 % Mn) areincluded in this group. Due to their high Si-content, decarburization and grain coarsening takes place inthese type of steels.
HEAT TREATMENT PROCEDURE (in general) :- Annealing : Slow & uniform heating in the range of 790- 800°C followed by furnace cooling at rate of 8-15°C/hr. Stress relieving : Heat to 650- 675°C and furnace cooling. Hardening : Preheating – warming to about 650°C & holding for 20 minutes/ 25mm. Austenitizing – heating to 900-950°C & holding again for 20minutes/25mm. Tempering : Heating to 205-650°C, holding for 30 minutes/25mm and then, air cooling.
HOT-WORKED TOOL STEELSCarbon content = 0.3-0.5% . These steels are used for hightemperature metal forming operation (except cutting), wherethe temperature is around 200-800°C.These are characterized by high hot yield strength, high redhardness , wear resistance, toughness, erosion resistance,resistance to softening at elevated temperatures, goodthermal conductivityThese are divided into 3 groups depending on the principlealloying elements: Chromium based [H11- H19] Tungsten based [H20- H26] Molybdenum based [H41- H43]
Chromium Based Contains Chromium (>=3.25%), and small amounts of Vanadium, Tungsten and Molybdenum. These are characterized by high red hardness & high hardenability. Oil quenching is reqd. when dimensional stability is not of prime importance. Tempering temperature for these steels varies from 550-675°C. Applications: Hot dies for extrusion, forging, mandrels, punches. Highly stressed structural parts of supersonic aircrafts. Hot work steels.
Tungsten Based Contains tungsten (=9.00%) & Chromium (2.0 -12.0%), and low Carbon %. These are characterized by resistance to high temperature softening. Tempering temperature for these steels varies from 550- 675°C. Applications: Punches . Mandrels . Extrusion dies for Brass, Steel & Nickel alloys.
Molybdenum Based Contains Molybdenum (8.00%) & Chromium (4.0 - 12.0%), and some tungsten and Vanadium. These are characterized by high toughness & high heat check resistance. Tempering temperature for these steels varies from 550- 650°C.
COLD-WORKED TOOL STEELSThese steels are used for making tools for cold workapplications, when the tool surface temperature does not risemore than 200°c.These are characterized by high abrasion & wearresistance, higher toughness and high impact resistance.These steels are also called “Non- distorting Steels”, as theyshow little change in dimension during heat treatment.These are divided into 3 groups: Oil hardening Steels [GRADE ‘O’] Air hardening Steels [GRADE ‘A’] High Carbon, High Chromium Steels [GRADE ‘D’]
Oil- hardening Steels These are hardened by oil-quenching & contain high carbon with manganese, chromium & molybdenum. These are characterized by high machinability, wear resistance & non-distorting properties. Tempering temperature for these steels varies from 100- 425°C. Applications: Taps . Blanking & forging dies. Threading dies. Expansion reamers.
Air- hardening Steels These are hardened by air-quenching and contain Carbon (1.0%) with manganese, chromium & molybdenum & tungsten. These are characterized by high wear resistance & high hardenability, fair red hardness, good toughness & resistance to decarburization. Tempering temperature for these steels varies from 150- 425°C. Applications: Knives . Blanking & trimming dies. Coining dies.
High carbon, high Chromium Steels These are hardened by oil- or air- hardening & contain Carbon (1.4-2.3%) & Chromium (12-14%), with molybdenum, cobalt, vanadium. Vanadium prevents these steels form showing Grain coarsening (upto 1040°C). Chromium imparts non-deforming properties. Tempering of these steels results in high hardness, wear & abrasion resistance. Tempering temperature for these steels varies from 150- 375°C. Applications: Mandrel for tube rolling by Pilger rolls . Blanking & piercing dies, Coining dies, Drawing dies.
HIGH SPEED TOOL STEELSThese are high alloyed tool steels developed initially to dohigh speed metal cutting. Now, they used in a wide variety ofmachining operations.These are characterized by high hardness (60-65 HRC at 600-650°C), high red hardness, wear resistance, reasonabletoughness and good hardenability.They contain 0.6 % carbon, 4% Chromium, 5-12% Cobalt.Carbon imparts hardness of at-least 60 HRC of martensiteformed. Chromium increase hardenability & corrosionresistance. Cobalt increases the thermal conductivity, meltingpoint, red hardness & wear resistance of high speed steels.
These are divided into two groups depending upon theprincipal alloying elements & the composition: Molybdenum High speed steel [GRADE ‘M’] (contain Molybdenum, Tungsten, Chromium, Vanadium & sometimes cobalt). Tungsten High Speed steels [GRADE ‘T’] (contain high amount of tungsten with chromium, vanadium and some cobalt.)Applications : End mills, drills, lathe tools, planar tools. Punches, reamers, Routers, taps, saws. Broaches, chasers, and hobs.
WATER-HARDENED TOOL STEELSThese steels contain carbon in the range of 0.9-1.0% alongwith Cr, V, Mo.These are characterized by high tensile strength & hardnesslevels but low ductility & toughness values.In order to improve machinability, these steels are given“Spheroidizing annealing treatment”.Presence of Cr improves both hardness & hardenability andVanadium checks the tendency of grain coarsening.Tempering temperatures are in the range 170-220°C.
Applications : Heavy forging hammers, hand hammers. Forging dies, bending dies, cutting dies. Large blanking tools, boring tools. Chisels, scissors, knife blades. Milling cutters, lathe centre. Watch maker’s tools. Engraving tools.